with generative adversarial networks
The MIT Faculty has made this article openly available.
how this access benefits you. Your story matters.
Mao, Yunwei et al., "Designing complex architectured materials with
generative adversarial networks." Science Advances 6, 17 (April
2020): eaaz4169 ©2020 Authors
American Association for the Advancement of Science (AAAS)
Final published version
Creative Commons Attribution NonCommercial License 4.0
Edisonian, and optimization, however, generally rely on experienced designers’ prior knowledge, limiting broad applications of architectured materials. Particularly challenging is designing architectured materials with extreme properties, such as the Hashin-Shtrikman upper bounds on isotropic elasticity in an experience- free manner without prior knowledge. Here, we present an experience-free and systematic approach for the design of complex architectured materials with generative adversarial networks. The networks are trained using simulation data from millions of randomly generated architectures categorized based on different crystallographic symmetries. We demonstrate modeling and experimental results of more than 400 two- dimensional architectures that approach the Hashin-Shtrikman upper bounds on isotropic elastic stiffness with porosities from 0.05 to 0.75.
Consisting of periodic arrays of truss, plate, and/or shell elements, architectured materials are ubiquitous in biological systems (1), structural engineering (2), and materials science (3) (Fig. 1). Archi-tectured materials have also found broad and important applications, such as light-weight structures (4, 5), thermal insulation (5), battery electrodes (6), optic and acoustic metamaterials (7, 8), and energy damping (9, 10). In addition, recent advances in additive manufacturing technologies such as three-dimensional (3D) printing have further made mass production of architectured materials with very complex structures feasible both technologically and economically.
Despite the important applications and great potential of archi-tectured materials, designing them is challenging. Existing designs of architectured materials generally follow approaches such as bioinspiration, Edisonian, theoretical analysis, and topology opti-mization. In the bioinspired approach, various naturally occurring biological structures such as honeycomb, trabecular bone, plant parenchyma, and sponge have been used as templates and inspirations for designing architectured materials for applications such as light-weight structural components (11), energy absorption (12), heat exchange (13), catalyst supports (14), filtration (15), and biomaterials (16). However, bioinspired designs usually do not guarantee optimal performances. In addition, many desired properties and functions of architectured materials cannot find counterparts in the biological system either. In the Edisonian approach, trial and errors in both experiments and simulations have been used to design Auxetic materials (17, 18), acoustic materials (19), phase-transformation materials (20), and kirigami shells for soft robots (21). The trial- and-error nature makes this approach not very efficient, and the resultant designs usually do not guarantee optimal performances either. Topology optimization uses gradient-based methods to reach architecture designs that give locally minimized/maximized properties.
This strategy has been widely used in designing architectured mate-rials with negative/zero thermal expansion (22, 23), multiscale porosity–induced high rigidity (24), and negative Poisson ratio (25). Despite its success and promise, topology optimization may suffer from the limitation of initial-guess dependence. The initial guess of the material topology can have an influence on the final design; different initial guesses may lead to different structures and properties (24, 26). Several theoretical analyses (27) of composites have helped understand the designs from the abovementioned approaches (28).
Furthermore, these traditional approaches usually require sub-stantial prior knowledge of experienced designers and provide limited numbers of designs. The challenge in designing architectured materials becomes particularly daunting when targeting at extreme properties such as designing configurations that reach the Hashin-Shtrikman (HS) upper bounds of isotropic elasticity and strain energy storage. For instance, so far, only a few classes of configurations that reach the HS upper bounds on isotropic elasticity in 2D via the topology optimization, such as coated spheres assemblages, rank-n laminates, Vigdergauz structures, and Sigmund structures (Fig. 2) (29).
Here, we present an experience-free and systematic approach for the design of complex architectured materials by harnessing machine- learning algorithms to analyze massive simulation data of randomly generated architectures categorized into different crystallographic symmetries. We first generate a set of data, composed of millions of configurations and their calculated properties, to represent the design space (Fig. 1A). We further categorize the dataset according to the crystallographic symmetries of the configurations. The data from selected crystallographic symmetries are then used to train the generative adversarial networks (GANs; Fig. 1B). In the GAN-based design, the discriminative network will map out the relationship between configurations and properties through learning the provided dataset. Meanwhile, armed with this knowledge on the relationship, the GANs are capable of promptly generating new configurations that approximately achieve the extreme properties (Fig. 1C). We demon-strate the capability of the proposed experience-free design with modeling and experimental results of more than 400 2D architectures that approach the HS upper bounds with porosities ranging from 0.05 to 0.75. This new design approach will not only facilitate the
1Department of Mechanical Engineering, Massachusetts Institute of Technology, Cambridge, MA 02139, USA. 2Department of Civil and Environmental Engineering, Massachusetts Institute of Technology, Cambridge, MA 02139, USA.
*These authors contributed equally to this work. †Corresponding author. Email: email@example.com
design of architectured materials (and structures in general) to achieve other extreme (or desired) properties but also shed light on a systematic method for various inverse designs. While neural networks have been used for structural optimization (30–32) and machine learning for the design of previously unknown composites (33, 34) and materials (35–37), the current work presents the design of complex architectured materials with GANs.
As illustrated in Fig. 3A, architectured materials consist of periodic arrays of units. A unit is composed of several identical elements, which undergo possible operations including reflect, rotate, and/or glide by following a specific crystallographic symmetry. Each element is discretized into a number of pixels that give a certain resolution of the element. A pixel can be in either solid or void phase, which is corresponding to the solid or void part in the architectured material, respectively. The porosity of an element (and the corresponding architectured material) is defined as the number of void pixels divided by the total number of pixels in the element. For example, Fig. 3A illustrates a 2D architectured material with p4 symmetry and the corresponding units, elements, and pixels.
There are 17 and 230 crystallographic symmetry groups in 2D and 3D spaces, respectively. For simplicity of conveying the key ideas of our method, we will focus on designs in 2D space in the current study. In Fig. 3B, we illustrate examples of units that follow the 17 symmetry groups in 2D. These symmetry groups have been characterized by mirror lines, fixed points, and/or glide lines to represent the reflect, rotate, and/or glide operations, respectively.
To generate the topology of an architectured material, we first generate the topology of its constituent element (e.g., gray part in Fig. 3B), map the element to a unit following a symmetry group, and then periodically translate the unit to form the architectured material. For a systematic design approach, the topology of the ele-ment needs to satisfy the following criteria: (i) the topology should be randomly generated to represent the whole design space; (ii) the number of the void pixels in an element should follow the assigned porosity; and (iii) the solid phase in the unit needs to be path- connected (38). Here, we develop an algorithm to generate the required configurations of elements. Briefly, we begin with an
element composed of all solid pixels and then randomly disperse voids with random size and shape to the element. Meanwhile, we guarantee that the remaining solid pixels are path-connected and that the total area of the voids follows the assigned porosity for the element. The details of our algorithm of random topology genera-tion are given in secgenera-tion S1.
Elastic constant calculation
Once the topology of an architectured material is generated (e.g., Fig. 3B), the finite element simulation is implemented to calculate the corresponding properties. For units with rectangular shape, the simulation domains are the units by themselves with periodic boundary conditions. For units with triangular and hexagonal shape, we map them into equivalent rectangular domains for simulation (39). In the calculation, we apply trial strain fields on the rectangular domain to obtain the reaction forces and the storage elastic energy. From the obtained reaction forces and the storage elastic energy, the equivalent constitutive behaviors of periodically patterned structures can be derived. Within the scope of linear elasticity, the equivalent constitutive behaviors of periodically patterned structures can be calculated using the homogenization method (40). By considering the first-order terms in the asymptotic expansion of the displacement field, it can be shown that the effective elastic tensor of the architec-tured materials ~ C ijkl can be expressed in the following form with the
Einstein index summation notation (23, 24, 41)
C ijkl = 1 ─S ∫ S C pqrs( ϵ 0(ij)pq − ϵ *(ij)pq ) ( ϵ rs0(kl) − ϵ rs*(kl) ) dS
where Cpqrs is the elastic tensor of the solid phase, ϵ pq0(ij) is the
ap-plied unit test strain, ϵ *(ij)pq is the fluctuation strain corresponding to
the unit test strain, and S is the area of the rectangular domain. Physically, the fluctuation strain is used to satisfy the periodic boundary condition for the rectangular domain, which is the periodic solution of
∫ S C ijpq ϵ pq*(kl) ∂ v ─∂ y i
j dS = ∫ S C ijpq ϵ pq
0(kl)─ ∂ v i
∂ y j dS
where v is a periodic admissible displacement field (23). After ~ C ijkl is
obtained, we can calculate the effective elastic properties (such as
Fig. 1. Schematics of procedures to design complex architectured materials. (A) Data generators to generate datasets of configurations and properties of architec-tured materials. (B) GANs trained by the datasets. (C) New designs of architecarchitec-tured materials with the targeted properties proposed by the GANs.
Young’s modulus, shear modulus, and Poisson’s ratio) of the ar-chitectured material along any direction. This method (41) has been broadly adopted in literature.
In many applications, it is desirable to achieve designs with isotropic properties. To guarantee the isotropy, the elastic constants, such as Young’s modulus ~ E , should be independent of the orientations of
the architectured materials. However, in reality, the perfect isotropy is difficult to achieve in architectured materials. To measure the isotropy of architectured materials, we follow the method given in (42, 43). We denote the maximum and minimum Young’s modulus in all possible directions of an architectured material with ~ E max and ~ E min , respectively (see Fig. 4A for an example).
The degree of isotropy can be defined as = ~ E / ~ E mean , where
~ E = _ ~ E max − ~ E min
2 and ~ E mean = _ ~ E max + ~ 2E min . We call the architectured
ma-terial nearly isotropic if ≤ 5%. This isotropic criterion is com-parable with or stricter than those used in the literature (42, 43).
After topology generation and properties calculation, we can con-struct 17 datasets corresponding to the 17 symmetry groups in 2D (note that 230 datasets can be generated corresponding to the 230 symmetry groups in 3D in the future). In each dataset, a data point is a combination of three items: pixel matrix for the element of an architectured material (fig. S3 and table S1), effective mean Young’s modulus ~ E mean of the architectured material, and isotropy of the
architectured material. The size of the dataset for each symmetry group is around one million configurations.
Machine learning algorithms
The datasets generated in previous sections will be used to train the GANs. GAN is a recently developed machine learning framework proposed to creatively generate complex outputs, such as fake faces, speeches, and videos (44). The adversarial structure can be composed of two competing deep neuron networks, a generative network and a discriminative network. In the GAN-based strategy, we use the
each symmetry group (~0.8 million) as the training set and keep the remaining 20% data (~0.2 million) as the testing set. All training details are discussed in section S2.
Achieving HS upper bounds
Next, we demonstrate the capability of the proposed approach to design architectured materials that approximately achieve the HS upper bounds of isotropic Young’s moduli. We first focus on designing architectures to achieve the HS upper bound at porosity = 0.5. Figure 4B shows the ranges of normalized mean Young’s moduli ~ E mean / E HS of nearly isotropic materials [ ≤ 5% (42, 43)]
generated in 17 crystallographic symmetries, where EHS = E(1 − )/
(1 + 2) is the theoretical HS upper Young’s modulus in 2D (46). It is noticeable that certain symmetries, i.e., p4, p4g, p3, p6, p3m1, p31m, and p6m, tend to give higher Young’s moduli in the training data-sets; and thus, these symmetries have higher potential to achieve the HS upper bound. For simplicity, we call these symmetries, i.e.,
p4, p4g, p3, p6, p3m1, p31m, and p6m, as high-potential symmetries.
Next, we use the datasets of the high-potential symmetries to train our GAN models. In Fig. 4D, we display 18 GAN-generated config-urations with = 0.5 and ≤ 5%, whose ~ E mean achieve more than
94% of EHS. Evidently, the maximum ~ E mean of architectures
gener-ated by the GAN in each symmetry group is higher than the range of the corresponding training dataset (Fig. 4B). This is consistent with the distributions of ~ E mean / E HS for the training dataset and for the
GAN outputs (Fig. 4C and fig. S16). This comparison shows that GANs can effectively extrapolate from the training data to provide multiple better designs than the randomly generated ones in each symmetry group. Notably, this design approach does not require any prior knowledge, bioinspiration, or trial-and-error iteration on the possible geometry of the architectured materials.
This experience-free design approach is widely applicable to other porosities. In Fig. 5A, we present a selected set of nearly isotropic configurations [ ≤ 5% (42, 43)], whose ~ E mean achieve more than
94% of EHS with porosities from 0.05 to 0.75. In figs. S5 to S15, we
further provide more than 360 additional nearly isotropic configu-rations that achieve more than 90% of EHS for a wide range of
porosities. The proximity of these configurations’ Young’s moduli to the HS upper bounds is comparable with or superior to that of previous designs in the literature (42, 43). While previous designs only gave a few configurations, the new capability of generating many desired configurations (e.g., more than 400) are impactful, due to two reasons. First, the proposed approach addresses a challenging inverse problem with multiple solutions in a systematic and experience- free manner. The proposed approach may also be useful for other inverse-design problems, such as designing architectured materials achieving the Suquet bound in plasticity (42). Second, if more constraints such as manufacturability were
Fig. 2. Four example classes of 2D structures designed with the topology op-timization that reach the HS upper bounds of isotropic elasticity and strain en-ergy storage. Adopted from (29).
imposed in practical applications, the multiple designs generated with the proposed approach would provide designers more choices for further selection.
We further demonstrate our design approach with experiments by fabricating GAN-generated architectured materials and measur-ing their Young’s moduli. Considermeasur-ing the requirement of isotropy of the solid phase, we choose to use laser-cut samples instead of 3D- printed ones. We measure the Young’s moduli of a number of proposed configurations with porosity from 0.05 to 0.75. For each porosity, three nearly isotropic architectures ( ≤ 5%) with the highest ~ E mean generated by GANs have been selected to fabricate
into testing samples. For the convenience of fabrication, the bound-aries between void phase and solid phase in the units are mapped to smooth curves with spline interpolation. Each unit is repeated three times in each direction to represent the periodic architec-tured material. Before performing experiments, finite element simulations are adopted to validate that the 3 × 3 units are suffi-cient to represent the periodic architectured materials and give the
effective Young’s moduli (see section S4 for details). Also, note that the 2D HS upper bound is defined under plane strain condi-tion. To mimic the plane strain condition, we adopt the con-strained uniaxial tension tests in the measurements (see section S4 for details). In Fig. 5B, we compare the Young’s moduli of a sample measured along various directions with the mean value of the measured Young’s moduli. The very mild deviations of the Young’s moduli from the mean value validate the near isotropy of the archi-tectured material.
In Fig. 5C, we summarize the experimentally measured effective mean Young’s moduli of various samples with porosities from 0.05 to 0.75. For each porosity, the samples are based on three nearly isotropic architectures ( ≤ 5%) generated by GANs with the high-est ~ E mean . We further compare the experimental results with the
theoretical HS upper bounds at various porosities. The measured effective mean Young’s moduli of GAN- generated nearly isotropic ( ≤ 5%) configurations can achieve more than 94% of the theoretical HS bound with porosities from 0.05 to 0.75.
Fig. 3. Illustrations of the pixel-wise architectured materials. (A) Definition of units, elements, and pixels in an architectured material. (B) Topology generation in 2D space by harnessing 17 groups of crystallographic symmetries. The porosity of architectures in (A) and (B) is set to be 0.5.
Here, we have proposed an experience-free and systematic approach for the design of complex architectured materials with GANs. The networks are trained using simulation data of millions of randomly
generated architectured materials categorized into different crystal-lographic symmetries. We demonstrate the capability of the proposed approach with modeling and experimental results of more than 400 2D architectures that approximately achieve the HS upper bounds of
Fig. 4. Architectured materials ( = 0.5) that approximate the HS bounds. (A) An example architecture and its Young’s Moduli in different directions. (B) Ranges of normalized Young’s Moduli ~ E mean / E HS ( ≤ 5%) of randomly generated architectures in 17 crystallographic symmetries. (C) The distributions of ~ E mean / E HS for the training dataset and for the GAN outputs (p6m, ≤ 5%) (D) Examples of GAN-generated architectured materials with ~ E mean ( ≤ 5 % ) achieving more than 94% of EHS. The nor-malized Young’s moduli of three highest ~ E mean ( ≤ 5%) generated by GANs in high-potential symmetries are marked as “×” in (B).
stiffness with porosities ranging from 0.05 to 0.75. While the pro-posed approach may take longer time to calculate the training datasets than the topology optimization, it represents an experience-free and systematic method that requires no prior knowledge and can be readily adopted in broad applications. In addition, the architectures generated in the current method can also serve as initial guess for
the further topology optimization if needed. This work not only provides a new method that harnesses simulation data and machine learning to potentially design future acoustic metamaterials (7, 8), auxetic materials (17, 18), and soft robotics (21) in an experience- free and systematic manner but also opens new avenues to addressing various inverse design problems in materials and structures.
Fig. 5. Architectured materials ( = 0.05 − 0.75) that approximate the HS bounds. (A) Examples of architectures with multiple porosities with ~ E mean ( ≤ 5 % ) achiev-ing more than 94% of EHS. (B) Photo of a laser-cut sample for an architecture and the measured Young’s moduli of the sample along various directions. (C) Comparison of ~ E mean of experimental samples and the theoretical HS upper bounds. The experimental samples are fabricated on the basis of three architectures generated by GANs with the highest ~ E mean ( ≤ 5%).
Structure of the GAN
The GAN consists of a generator and a discriminator. The generator is composed of five layers of neural networks. The first layer is a fully connected layer composed of 1024 neurons to receive the data from the database. The second layer is also a fully connected layer composed of 1600 neurons. The third and fourth layers are convo-lutional layers composed of 64 and 32 neurons, respectively. The last layer is a deconvolutional layer associated with a tanh activa-tion funcactiva-tion to produce configuraactiva-tions with bounded pixel values. The discriminator is composed of three layers of neural networks. The first and second layers are convolutional layers composed of 64 and 128 neurons, respectively. Their convolutional window size is set to be 4 × 4. The first convolutional layer is associated with batch normalization operations and leaky rectified linear unit acti-vations, and the second convolutional layer has a sigmoid activation function to produce probabilities between 0 and 1. The second layer has been flattened, and the output of the second layer is sent to the third layer, which is a fully connected layer composed of 1024 neurons.
The total loss is composed of the adversarial loss and the style transfer loss. The adversarial loss is for the minimum-maximum training process of GAN, and the style transfer loss enables the porosity of the generated configuration to approach the target porosity. The weight of the style transfer loss is set to be 0.03 to prevent the style transfer loss from diminishing to zero or over-whelming the GAN adversarial loss. The Adam optimizer is applied in training by setting the learning rate as 0.0001. The batch size for training is set to be 32.
Fabrication of architectured materials
The pixel-wise architectures generated by GANs were first imported into the sketch module of SOLIDWORKS to smooth the solid-void boundaries by the cubic spline interpolation. Thereafter, each ar-chitecture was uploaded to the laser cutter (Epilog Mini/Helix; Epilog Laser), which cut an acrylic plate multiple times with minimal laser energy. The resultant testing sample has overall dimensions of 50 mm by 50 mm by 2.25 mm. A constrained uniaxial tensile test was carried out on the sample to obtain the stress-strain curve.
Supplementary material for this article is available at http://advances.sciencemag.org/cgi/ content/full/6/17/eaaz4169/DC1
REFERENCES AND NOTES
1. S. A. Wainwright, W. D. Biggs, J. D. Currey, Mechanical Design in Organisms (Princeton University Press, 1982).
2. A. G. Evans, J. W. Hutchinson, N. A. Ashby, H. N. G. Wadley, The topological design of multifunctional cellular metals. Prog. Mater. Sci. 46, 309–327 (2001).
3. L. J. Gibson, M. F. Ashby, Cellular Solids: Structure and Properties (Cambridge University Press, 1999).
10. L. Salari-Sharif, T. A. Schaedler, L. Valdevit, Energy dissipation mechanisms in hollow metallic microlattices. J. Mater. Res. 29, 1755–1770 (2014).
11. L. Valdevit, A. J. Jacobsen, J. R. Greer, W. B. Carter, Protocols for the optimal design of multi-functional cellular structures: From hypersonics to micro-architected materials. J. Amer. Ceramics Soc. 94, s15–s34 (2011).
12. T. A. Schaedler, C. J. Ro, A. E. Sorensen, Z. Ecke, S. S. Yang, W. B. Carter, A. J. Jacobsen, Designing metallic microlattices for energy absorber applications. Adv. Eng. Mater. 16, 276–283 (2013).
13. L. Valdevit, A. Pantano, H. A. Stone, A. G. Evans, Optimal active cooling performance of metallic sandwich panels with prismatic cores. Int. J. Heat Mass Trans. 49, 3819–3830 (2006).
14. O.-Y. Kwon, H.-J. Ryu, S.-Y. Jeong, Porous layered carbon as catalyst support material for PEMFC. J. Industrial Engr. Chem. 12, 306–310 (2006).
15. R. A. Oslon III, L. C. B. Martins et al., Adv. Eng. Mater. 7, 16 (2005).
16. S. Baudis, F. Nehl, S. C. Ligon, H. Bergmeister, D. Bernhard, J. Stampfl, R. Liska, Elastomeric degradable biomaterials by photopolymerization-based CAD-CAM for vascular tissue engineering. Biomed. Mater. 6, 055003 (2011).
17. S. Babaee, J. Shim, J. C. Weaver, E. R. Chen, N. Patel, K. Bertoldi, 3D soft metamaterials with negative poisson’s ratio. Adv. Mater. 25, 5044–5049 (2013).
18. K. Bertoldi, P. M. Reis, S. Willshaw, T. Mullin, Negative Poisson’s ratio behavior induced by an elastic instability. Adv. Mater. 22, 361–366 (2010).
19. P. Wang, F. Casadei, S. Shan, J. C. Weaver, K. Bertoldi, Harnessing buckling to design tunable locally resonant acoustic metamaterials. Phys. Rev. Lett. 113, 014301 (2014). 20. T. Mullin, S. Deschanel, K. Bertoldi, M. C. Boyce, Pattern transformation triggered by
deformation. Phys. Rev. Lett. 99, 084301 (2007).
21. A. Rafsanjani, L. Jin, B. Deng, K. Bertoldi, Propagation of pop ups in kirigami shells. Proc. Natl. Acad. Sci. U.S.A. 116, 6 (2019).
22. O. Sigmund, S. Torquato, Composites with extremal thermal expansion coefficients. Appl. Phys. Lett. 69, 3203 (1996).
23. O. Sigmund, S. Torquato, Design of materials with extreme thermal expansion using a three-phase topology optimization method. J. Mech. Phys. Solids 45, 1037–1067 (1997).
24. X. Liang, P. Breitkopf, Concurrent topology optimization design of material and structure
within FE2 nonlinear multiscale analysis framework. Comput. Methods Appl. Mech. Eng.
278, 524–542 (2014).
25. S. Amstutz, S. M. Giusti, A. A. Novotny, E. A. de Souza Neto, Topological derivative for multi-scale linear elasticity models applied to the synthesis of microstructures. Int. J. Numer. Methods Eng. 84, 733–756 (2010).
26. M. P. Bense, O. Sigmund, Topology Optimization Theory, Method and Applications (Springer, 2003).
27. G. W. Milton, A. T. Sawicki, Theory of composites. Cambridge monographs on applied and computational mathematics. Appl. Mech. Rev. 56, B27–B28 (2003).
28. G. W. Milton, Composite materials with Poisson’s ratios close to—1. J. Mech. Phys. Solids 40, 1105–1137 (1992).
29. O. Sigmund, A new class of extremal composites. J. Mech. Phys. Solids 48, 397–428 (2000).
30. M. Papadrakakis, N. D. Lagaros, Y. Tsompanakis, Structural optimization using evolution strategies and neural networks. Comput. Methods Appl. Mech. Eng. 156, 309–333 (1998). 31. M. Papadrakakis, N. D. Lagaros, G. Thierauf, J. Cai, Advanced solution methods
in structural optimization based on evolution strategies. Engr. Comput. 15, 12–34 (1998). 32. M. Papadrakakis, N. D. Lagaros, Reliability-based structural optimization using neural
networks and Monte Carlo simulation. Comput. Methods Appl. Mech. Eng. 191, 3491–3507 (2002).
33. G. Gu, C.-T. Chen, M. J. Buehler, De novo composite design based on machine learning algorithm. Extreme Mech. Lett. 18, 19–28 (2018).
34. G. Gu, C.-T. Chen, D. J. Richmond, M. J. Buehler, Bioinspired hierarchical composite design using machine learning: Simulation, additive manufacturing, and experiment. Mater. Horizons 5, 939–945 (2018).
35. R. Liu, A. Kumar, Z. Chen, A. Agrawal, V. Sundararaghavan, A. Choudhary, A predictive machine learning approach for microstructure optimization and materials design. Sci. Rep. 5, 11551 (2015).
36. Y. Liu, T. Zhao, W. Ju, S. Shi, Materials discovery and design using machine learning. J. Materiomics 3, 159–177 (2017).
37. P. Hanakata, E. D. Cubuk, D. K. Campbell, H. S. Park, Accelerated search and design of stretchable graphene kirigami using machine learning. Phys. Rev. Lett. 121, 255304 (2018).
38. S. Lefschetz, Introduction to Topology (Princeton University Press, 2015). 39. W. D. Callister, D. G. Rethwisch, Materials Science and Engineering: An Introduction
(John Wiley & Sons, 2007), vol. 7.
40. D. Schattschneider, The plane symmetry groups: Their recognition and notation. Amer. Math. Monthly 85, 439–450 (1978).
41. K. Suzuki, N. Kikuchi, A homogenization method for shape and topology optimization. Comput. Methods Appl. Mech. Eng. 93, 291–318 (1991).
42. T. Tancogne-Dejean, M. Diamantopoulou, M. B. Gorji, C. Bonatti, D. Mohr, 3D plate-lattices: An emerging class of low-density metamaterial exhibiting optimal isotropic stiffness. Adv. Mater. 30, e1803334 (2018).
43. J. B. Berger, H. N. G. Wadley, R. M. McMeeking, Mechanical metamaterials at the theoretical limit of isotropic elastic stiffness. Nature 543, 533–537 (2017). 44. I. Goodfellow, J. Pouget-Abadie, M. Mirza, B. Xu, D. Warde-Farley, S. Ozair, A. Courville,
Y. Bengio, Generative adversarial nets, in Advances in Neural Information Processing Systems (NIPS, 2014).
45. M. Abadi, P. Barham, J. Chen, Z. Chen, A. Davis, J. Dean, M. Devin, S. Ghemawat, G. Irving, M. Isard, M. Kudlur, J. Levenberg, R. Monga, S. Moore, D. G. Murray, B. Steiner, P. Tucker,
V. Vasudevan, P. Warden, M. Wicke, Y. Yu, and X. Zheng, Tensorflow: A system for large-scale machine learning, in 12th USENIX Symposium on Operating Systems Design and Implementation OSDI 16 (2016).
46. Z. Hashin, On elastic behaviour of fibre reinforced materials of arbitrary transverse phase geometry. J. Mech. Phys. Solids 13, 119–134 (1965).
Funding: This work was supported by the NSF (EFMA-1935291) and the U.S. Army Research Office through the Institute for Soldier Nanotechnologies at Massachusetts Institute of Technology (W911NF-13-D-0001). Author contributions: Y.M., Q.H., and X.Z. conceived the idea, designed the study, and interpreted the results. Y.M. and Q.H. programed the codes for the topology generator and machine learning setup. Y.M. and Q.H. performed experimental measurement. Y.M., Q.H., and X.Z. drafted the manuscript. X.Z. supervised the study. Q.H. thanks S. Lin for help in experiments. Competing interests: The authors declare that they have no competing interests. Data and materials availability: All data needed to evaluate the conclusions in the paper are present in the paper and/or the Supplementary Materials. Additional data related to this paper may be requested from the authors. Submitted 6 September 2019
Accepted 27 January 2020 Published 24 April 2020 10.1126/sciadv.aaz4169
Citation: Y. Mao, Q. He, X. Zhao, Designing complex architectured materials with generative adversarial networks. Sci. Adv. 6, eaaz4169 (2020).